- Nano Express
- Open Access
Enhanced Power Conversion Efficiency of Perovskite Solar Cells with an Up-Conversion Material of Er3+-Yb3+-Li+ Tri-doped TiO2
Nanoscale Research Letters volume 13, Article number: 147 (2018)
In this paper, Er3+-Yb3+-Li+ tri-doped TiO2 (UC-TiO2) was prepared by an addition of Li+ to Er3+-Yb3+ co-doped TiO2. The UC-TiO2 presented an enhanced up-conversion emission compared with Er3+-Yb3+ co-doped TiO2. The UC-TiO2 was applied to the perovskite solar cells. The power conversion efficiency (PCE) of the solar cells without UC-TiO2 was 14.0%, while the PCE of the solar cells with UC-TiO2 was increased to 16.5%, which presented an increase of 19%. The results suggested that UC-TiO2 is an effective up-conversion material. And this study provided a route to expand the spectral absorption of perovskite solar cells from visible light to near-infrared using up-conversion materials.
Organolead halide perovskite solar cells (PSCs) have become attractive in the solar cell field, which is due to their advantages, such as high efficiency, lost cost, and simple fabrication [1,2,3,4]. In a few years, the power conversion efficiency (PCE) of PSCs has been improved to 22.1% . However, perovskite solar cells only absorb a small fraction of incident light in UV and visible ranges due to the narrow energy band gap of perovskite sensitizer; thus, a large portion of incident light is lost due to its non-absorption of near-infrared (NIR) [6, 7].
One promising method to solve the NIR energy loss issue is to apply up-conversion materials to PSCs, which can convert NIR to visible light. Some authors have reported the applications of up-conversion materials to perovskite solar cells [8,9,10], in which the up-conversion materials adopted were mainly based on beta-phase sodium yttrium fluoride (β-NaYF4). While the β-NaYF4 up-conversion materials can reduce charge transport ability of electron transfer layer . It has been reported that Er3+-Yb3+-F− tri-doped TiO2 can improve the PCE of dye-sensitized solar cells (DSSCs) due to its enhanced up-conversion emission compared with Er3+-Yb3+ co-doped TiO2 . In our previous publication , we reported the application of Er3+-Yb3+ co-doped TiO2 nanorods to PSCs. Some researchers have proved that the addition of Li+ into Er3+-Yb3+ co-doped TiO2 could increase the up-conversion emission [14, 15]. And it has been reported that the perovskite solar cells based on Li-doped TiO2 produce higher performances compared to the device based on un-doped TiO2 . Thus, we wonder if the up-conversion materials of Er3+-Yb3+-Li+ tri-doped TiO2 can be applied to PSCs to further improve the performance.
Therefore, in the present study, we prepared Er3+-Yb3+-Li+ tri-doped TiO2 (UC-TiO2) by addition of Li+ into Er3+-Yb3+ co-doped TiO2, which presented an enhanced up-conversion emission compared with Er3+-Yb3+ co-doped TiO2. The UC-TiO2 was applied to perovskite solar cells. The PCE of the solar cells with UC-TiO2 is increased to 16.5 from 14.0% for the solar cells without UC-TiO2, which presents an increase of 19%.
Synthesis of Er3+-Yb3+-Li+ Tri-Doped TiO2
The nanocrystals of Er3+-Yb3+-Li+ tri-doped TiO2 (UC-TiO2) were synthesized by a modified method . A titanium (IV) n-butoxide was prepared by mixing n-butyl titanate (Ti(OBu)4) with acetylacetone (AcAc) at room temperature for 1 h under agitation. Then, the iso-propyl (i-PrOH) was put in the titanium (IV) n-butoxide. Next, i-PrOH, deionized water, and concentrated nitric acid (HNO3) was mixed and dropped into the solution. A light yellow TiO2 sol was obtained after stirring for 6 h. The molar ratios of AcAc, H2O, and HNO3 to Ti(OBu)4 were 1:1, 2:1, and 0.3:1, respectively. Then, Er(NO3)3·5H2O, Yb(NO3)3·5H2O, and LiNO3 were added into the TiO2 sol to make the molar ratios of Er:Yb:Li:Ti = 0.5:10:x:100 (x = 0, 10, 15, 20, 25). The solvent in the Er3+-Yb3+-Li+ tri-doped TiO2 sol (UC-TiO2 sol) was removed by drying for 8 h at 100 °C. Then, the UC-TiO2 was calcined at 500 °C for 30 min.
Fabrication of Perovskite Solar Cells
Patterned FTO glass substrate was cleaned in acetone, 2-propanol, and ethanol by sonication for 20 min, respectively. Then, UV-O3 was used to treat the FTO for 15 min. A compact layer was formed by spin-coating a precursor solution on FTO and annealed at 500 °C for 30 min. The precursor solution is 0.1 M titanium diisopropoxide bis (acetylacetonate) (75 wt% in isopropanol, Aldrich) solution in 1-butanol. A mesoporous TiO2 film was obtained by spin-coating TiO2 solution on the compact layer at 4000 rpm for 30 s, followed by annealing at 100 °C for 10 min and 500 °C for 30 min, respectively. The TiO2 solution was prepared by diluting TiO2 paste (30NR-D, Dyesol) with ethanol (1:6, weight ratio) or by mixing the UC-TiO2 sol and the diluted TiO2 solution (UC-TiO2:TiO2 = x:100, v/v, x = 10, 20, 30, and 40). A perovskite layer was formed on UC-TiO2 layer by spin-coating perovskite precursor solution in two steps at 1000 rpm for 10 s and 4000 rpm for 30 s, and 200 μL chlorobenzene was poured on the substrate during the second step before the end of 20 s. Then, the sample was heated on the hotplate at 100 °C for 1 h. The perovskite precursor solution was obtained by mixing PbI2 (1.1 M), FAI (1 M), PbBr2 (0.22 M), and MABr (0.2 M) in the mixed solvent of anhydrous DMF/DMSO (4:1 v:v). Then, a 1.5 M stock solution of CsI pre-dissolved in DMSO was dropped into the mixed perovskite precursor solution . A hole-transfer layer was formed by spin-coating a solution of spiro-MeOTAD at 4000 rpm 30 s. Finally, an 80-nm-thick gold layer was thermally evaporated on the top of the device.
Up-conversion fluorescence, steady-state photoluminescence (PL), and time-resolved photoluminescence (TRPL) spectra were measured with a FLS 980 E fluorometer (Edinburgh Photonics). X-ray diffraction (XRD) spectra were acquired on a diffractometer (DX-2700). X-ray photoelectron spectroscopy (XPS THS-103) with Al Ka as X-ray source was applied to measure the chemical state of the samples. Ultraviolet visible near-infrared (UV-vis-NIR) absorption spectra were collected on a Varian Cary 5000 spectrophotometer. Microstructure and morphologies were observed with a scanning electron microscope (SEM; JEM-7001F, JEOL). Photocurrent-voltage (J-V) curves were measured with a Keithley 2440 Sourcemeter under AM 1.5 G illumination. The electrochemical impedance spectroscopy (EIS) was obtained with an electrochemical workstation (CHI660e, Shanghai CHI Co., Ltd.).
Results and Discussion
Up-conversion emissions were measured with an excitation of a 980-nm laser. Figure 1a shows the up-conversion emissions spectra of Er3+-Yb3+-Li+ tri-doped TiO2 (Er:Yb:Li:Ti = 0.5:10:x:100, x = 0, 10, 15, 20, and 25, molar ratio). Figure 1b shows the schematic energy-transfer mechanisms of the Er3+ ions. The green emission bands located at about 525 and 545 nm can be attributed to 2H11/2→4I15/2 and 4S3/2→4I15/2 transitions of Er3+ ions, respectively. And the red emission bands centered at about 658 nm could correspond to 4F9/2→4I15/2 transitions of Er3+ ions [15, 16]. With the increase of Li+ doping content, the intensity of the spectrum increases firstly, and then decreases, which is the maximum when the doping content of Li+ is x = 20. Hereinafter, the up-conversion material of Er3+-Yb3+-Li+ tri-doped TiO2 (Er:Yb:Li:Ti = 0.5:10:20:100, molar ratio) was applied.
Figure 2 displays the XRD patterns of commercial TiO2 (30NR-D) and UC-TiO2. The XRD pattern of UC-TiO2 is similar to that of 30NR-D. The peaks at 25.3°, 37.8°, 48.0°, and 53.8° in the XRD patterns are assigned to the (101), (004), (200), and (105) planes (JCPDS card no.21-1272), respectively, which indicates that UC-TiO2 and 30NR-D belong to the anatase phase of TiO2.
To confirm the doping of Er, Yb, and Li into TiO2, XPS spectra of UC-TiO2 were recorded and shown in Fig. 3. The peaks at 458.1 and 463.9 eV in Fig. 3a could belong to Ti 2p3/2 and Ti 2p1/2, respectively, and the peaks at 168.8 eV in Fig. 3b and at 192.7 eV in Fig. 3c could be attributed to Er 4d and Yb 4d, respectively . The peak at 55.5 eV in Fig. 3d can correspond to Li 1s . The survey XPS spectrum of UC-TiO2 and O1s peak were also presented in Additional file 1: Figure S1. The results demonstrated that Er, Yb, and Li atoms were doped into TiO2.
Figure 4a displays the UV-vis-NIR absorption spectra of TiO2 (30NR-D) and UC-TiO2. Compared with 30NR-D, UC-TiO2 presents a stronger absorption, especially at the range from 900 to 1000 nm. The energy band gap (Eg) could be estimated with the Tauc plot . The Tauc plots are shown in Fig. 4b, from which the values of Eg could be obtained to be 3.20 and 3.10 eV for 30NR-D and UC-TiO2, respectively. The Eg of UC-TiO2 is smaller than that of un-doped TiO2.
Figure 5a shows the SEM image of 30NR-D film formed on the compact layer. The nanoparticle size is about 30 nm, and the size distribution is uniform. Figure 5b shows the SEM image of the film containing 30NR-D and UC-TiO2 deposited on the compact layer by spin-coating method. There is no obvious difference between the two films, which displays that the particle size and morphology of UC-TiO2 are similar to those of 30NR-D.
In the present work, the perovskite film was formed with the method previously reported . According to report, the composition of the perovskite film is Cs5(MA0.17FA0.83)95Pb(I0.83Br0.17)3, and the role of the CsI is to make the perovskite solar cells thermally more stable, with less phase impurities, and less sensitive to processing conditions . The scheme of the device is presented in Additional file 1: Figure S2.
The perovskite solar cells based on mesoporous layer formed with the mixture of UC-TiO2 sol and diluted TiO2 solution (UC-TiO2:TiO2 = x:100, v/v, x = 0, 10, 20, 30, and 40) were fabricated and their I-V curves were measured. The photovoltaic parameters were obtained from the I-V measurements. Figure 6a shows the PCE dependence of solar cells on the content of UC-TiO2 (UC-TiO2:TiO2 = x:100, v/v) in the mixture. With the increase of UC-TiO2 content, the power conversion efficiency (PCE) of solar cells increases firstly, and then decreases, which is the maximum at the content of x = 20 for UC-TiO2. The detailed photovoltaic parameters of solar cells with 20% UC-TiO2 and without UC-TiO2 were listed in Table 1. Compared with those of the devices without UC-TiO2, the photovoltaic parameters of the solar cells with UC-TiO2 present an improvement. The PCE of the solar cells with 20% UC-TiO2 is increased to 16.5 from 14.0% for the solar cells without UC-TiO2, which presents an increase of 19%. Figure 6b displays the I-V curves of the typical solar cells with UC-TiO2 and without UC-TiO2.
To understand the enhancement, some investigations were carried out. Steady-state photoluminescence (PL) and time-resolved photoluminescence (TRPL) can be applied to investigate the electron extration and transport process. The PL of perovskite layer on the mesoporous layers formed by 30NR-D and 30NR-D with UC-TiO2 were measured and shown in Fig. 7a. Compared with that of 30NR-D/perovskite, the PL intensity of 30NR-D with UC-TiO2/perovskite becomes reduced, which indicates that the electron extration and transport efficiency across the interface between 30NR-D with UC-TiO2 and perovskite is better than that between 30NR-D and perovskite . Figure 7b shows the TRPL spectra of perovskite layer on the mesoporous layers formed by 30NR-D and 30NR-D with UC-TiO2. The TRPL spectrum was fitted to a biexponential function, in which the fast decay (τ1) may be resulted from transportation of free carriers, and the slow decay (τ2) can be originated from radiative recombination of free carriers [22,23,24]. The obtained parameters are listed in Table 2. Compared with that of 30NR-D/perovskite, the fast decay time (2.8 ns) of 30NR-D with UC-TiO2/perovskite becomes smaller, while the fraction of fast decay process (98.2%) becomes larger. This implies that the charge transfer between perovskite and 30NR-D with UC-TiO2 is faster than that between perovskite and 30NR-D.
Eletrochemical impedance spectroscopy (EIS) is an effective method to get some information on carrier transfer behavior. Figure 8a displays the Nyquist plots of the devices based on mesoporous layers formed by 30NR-D and 30NR-D with UC-TiO2, in which two arcs were observed. The arc at high-frequency could be resulted from the contact resistance between the interfaces, and the arc at low-frequency could come from the recombination resistance (Rrec) and chemical capacitance (Cμ) of the device [25, 26]. The EIS was fitted with an equivalent circuit shown in Fig. 8b, and the obtained parameters are listed in Table 3. The series resistance of the devices based on 30NR-D with UC-TiO2 becomes smaller than that of the devices on based on 30NR-D, while the recombination resistance of the former becomes larger than that of the later. This indicates the charge recombination was decreased and the charge transport was improved for the device based on 30NR-D with UC-TiO2.
To further prove the effect of UC-TiO2 on photocurrents of the devices, the I-V curves of the devices based on the mesoporous layers without UC-TiO2 and with UC-TiO2 were measured under the simulated solar radiation in the wavelength range of λ ≥ 980 nm with a NIR filter, which are shown in Additional file 1: Figure S3. Compared with that of the device without UC-TiO2, the photocurrent of the device with UC-TiO2 was obviously enhanced, which demonstrates that the incorporation of UC-TiO2 in the device can transform the NIR light into visible light, which can be absorbed by the devices to generate photocurrent.
To explain the increased open circuit voltage (Voc) of the solar cells, the energy band arrangements of UC-TiO2, TiO2, perovskite, and Spiro-OMeTAD were shown in Fig. 9 based on the absorption spectra (Fig. 4) and the literatures [27, 28]. The conduction band edge of the UC-TiO2 is lower than that of TiO2 (30NR-D) due to its smaller energy band gap; thus, the conduction band offset between UC-TiO2 and perovskite is larger than that between TiO2 and perovskite. This could be one of the reasons to have a higher open circuit voltage for UC-TiO2 based solar cells [29, 30].
In summary, the PCE increase of the solar cells based on the mesoporous layer with UC-TiO2 is due to the enlarged Isc and increased Voc. The enlarged Isc could be due to expansion of spectral absorption to near-infrared (NIR) range with up-conversion material, reduced recombination, and fast charge transfer of photo-generated carriers. The increased Voc may be attributed to the enlarged conduction band offset between UC-TiO2 and perovskite.
Er3+-Yb3+-Li+ tri-doped TiO2 (UC-TiO2) was prepared by addition of Li+ into Er3+-Yb3+ co-doped TiO2, which presented an enhanced up-conversion emission. The UC-TiO2 was applied to the perovskite solar cells. The performance of solar cells with UC-TiO2 was improved compared with that of control device. The Isc, Voc, and FF of solar cells with UC-TiO2 were increased to 22.2 mA/cm2, 1.05 V, and 70.8% from 21.0 mA/cm2, 1.01 V, and 66.0% for the control devices, respectively. Thus, the PCE with UC-TiO2 was increased to 16.5 from 14.0% for the solar cells without UC-TiO2, which presents an increase of 19%. Based on some experimental results, this PCE increase was explained.
Electrochemical impedance spectroscopy
Power conversion efficiency
Perovskite solar cells
Ahn N, Son DY, Jang IH, Kang SM, Choi M, Park NG (2015) Highly reproducible perovskite solar cells with average efficiency of 18.3% and best efficiency of 19.7% fabricated via Lewis base adduct of lead(II) iodide. J Am Chem Soc 137:8696–8699
McMeekin DP, Sadoughi G, Rehman W, Eperon GE, Saliba M, Horantner MT, Haghighirad A, Sakai N, Korte L, Rech B, Johnston MB, Herz LM, Snaith HJ (2016) A mixed-cation lead mixed-halide perovskite absorber for tandem solar cells. Science 351:151–155
Tsai H, Nie WY, Blancon JC, Toumpos CC, Asadpour R, Harutyunyan B, Neukirch AJ, Verduzco R, Crochet JJ, Tretiak S, Pedesseau L, Even J, Alam MA, Gupta G, Lou J, Ajayan PM, Bedzyk MJ, Kanatzidis MG, Mohite AD (2016) High-efficiency two-dimensional Ruddlesden-Popper perovskite solar cells. Nature 536:312–316
Arora N, Dar MI, Hinderhofer A, Pellet N, Schreiber F, Zakeeruddin SM, Gratzel M (2017) Perovskite solar cells with CuSCN hole extraction layers yield stabilized efficiencies greater than 20%. Science 358:768–771
Yang WS, Park BW, Jung EH, Jeon NJ, Kim YC, Lee DC, Shin SS, Seo J, Kim EK, Noh JH, Seok SI (2017) Iodide management in formamidinium lead halide based perovskite layers for efficient solar cells. Science 356:1376–1379
Liu MZ, Johnston MB, Snaith HJ (2013) Efficient planar heterojunction perovskite solar cells by vapour deposition. Nature 501:395–398
Zhang JB, Xu B, Johansson MB, Vlachopoulos N, Boschloo G, Sun LC, Johansson EMJ, Hagfeldt A (2016) Strategy to boost the efficiency of mixed-ion perovskite solar cells: changing geometry of the hole transporting material. ACS Nano 10:6816–6825
He M, Pang XC, Liu XQ, Jiang BB, He YJ, Snaith H, Lin ZQ (2016) Monodisperse dual-functional upconversion nanoparticles enabled near-infrared organolead halide perovskite solar cells. Angew Chem Int Ed 55:4280–4284
Roh JM, Yu HJ, Jang J (2016) Hexagonal β-NaYF4:Yb3+, Er3+ nanoprism incorporated upconverting layer in perovskite solar cells for near-infrared sunlight harvesting. ACS Appl Mater Interfaces 8:19847–19852
Que M, Que W, Yin X, Chen P, Yang Y, Hu J, Yu B, Du Y (2016) Enhanced conversion efficiency in perovskite solar cells by effectively utilizing near infrared light. Nano 8:14432–14437
Yu J, Yang Y, Fan R, Liu DQ, Wei LG, Chen S, Li L, Yang B, Cao WW (2014) Enhanced near-infrared to visible upconversion nanoparticles of Ho3+-Yb3+-F− tri-doped TiO2 and its application in dye-sensitized solar cells with 37% improvement in power conversion efficiency. Inorg Chem 53:8045–8053
Yu J, Yang YL, Fan RQ, Zhang HJ, Li L, Wei LG, Shi Y, Pan K, Fu HG (2013) Er3+ and Yb3+ co-doped TiO2-xFx up-conversion luminescence powder as a light scattering layer with enhanced performance in dye sensitized solar cells. J Power Sources 243:436–443
Wang XL, Zhang ZL, Qin JQ, Shi WJ, Liu YF, Gao HP, Mao YL (2017) Enhanced photovoltaic performance of perovskite solar cells based on Er-Yb co-doped TiO2 nanorod arrays. Electrochim Acta 245:839–845
Cao BS, He YY, Sun Y, Song M, Dong B (2011) Optical high temperature sensor based on enhanced green upconversion emissions in Er3+-Yb3+-Li+ codoped TiO2 powders. J Nanosci Nanotechnol 11:9899–9903
He YY, Wu JL, Wang XH, Feng ZQ, B. Dong B. (2016) Optical temperature sensing behavior through stark sublevels transitions of green and red upconversion emissions for Er3+-Yb3+-Li+ codoped TiO2 phosphors. J Nanosci Nanotechnol 16:3768–3771
Giordano F, Abate A, Baena JPC, Saliba M, Matsui T, Im SH, Zakeeruddin SM, Nazeeruddin MK, Hagfeldt A, Graetzel M (2015) Enhanced electronic properties in mesoporous TiO2 via lithium doping for high-efficiency perovskite solar cells. Nat Commun 7:10379
Michael S, Taisuke M, Seo JY, Domanski K, Correa-Baena JP, Nazeeruddin MK, Zakeeruddin SM, Tress W, Abate A, Hagfeldtd A, Gratzel M (2016) Cesium-containing triple cation perovskite solar cells: improved stability, reproducibility and high efficiency. Energy Environ Sci 9:1989–1997
Ji TH, Liu Y, Zhao H, Du HY, Sun JY, Ge GL (2010) Preparation and up-conversion fluorescence of rare earth (Er3+ or Yb3+/Er3+)-doped TiO2 nanobelts. J Solid State Chem 183:584–589
Ravishankar TN, Nagaraju G, Dupont J (2016) Photocatalytic activity of Li-doped TiO2 nanoparticles: synthesis via ionic liquid-assisted hydrothermal route. Mater Res Bull 78:103–111
Gao XX, Ge QQ, Xue DJ, Ding J, Ma JY, Chen YX, Zhang B, Feng YQ, Wan LJ, Hu JS (2016) Tuning the fermi-level of TiO2 mesoporous layer by lanthanum doping towards efficient perovskite solar cells. Nano 8:16881–16885
Liang C, Wu Z, Li P, Fan JJ, Zhang YQ, Shao GS (2016) Chemical bath deposited rutile TiO2 compact layer toward efficient planar heterojunction perovskite solar cells. Appl Surf Sci 391:337–344
Chen Q, Zhou H, Song TB, Luo S, Hong Z, Duan HS, Dou L, Liu Y, Yang Y (2014) Controllable self-induced passivation of hybrid lead iodide perovskites toward high performance solar cells. Nano Lett 14:4158–4163
Liang PW, Liao CY, Chu CC, Zuo F, Williams ST, Xin XK, Lin J, Jen AKY (2014) Additive enhanced crystallization of solution-processed perovskite for highly efficient panar-heterojunction solar cells. Adv Mater 26:3748–3754
Yeo JS, Kang R, Lee SY, Jeon YJ, Myoung NS, Lee CL, Kim DU, Yun JM, Seo YH, Kim SS, Na SI (2015) Highly efficient and stable planar perovskite solar cells with reduced grapheme oxide nanosheets as electrode interlayer. Nano Energy 12:96–104
Liu DY, Yang JL, Kelly TL (2014) Compact layer free perovskite solar cells with 13.5% efficiency. J Am Chem Soc 136:17116–17122
Kim HS, Lee JW, Yantara N, Boix PP, Kulkarni SA, Mhaisalkar S, Gratzel M, Park NG (2013) High efficiency solid-state sensitized solar cell-based on submicrometer rutile TiO2 nanorod and CH3NH3PbI3 perovskite sensitizer. Nano Lett 13:2412–2417
Rhee JH, Chung CC, Diau WG (2013) A perspective of mesoscopic solar cells based on metal chalcogenide quantum dots and organometal-halide perovskites. NPG Asia Mater 5:e68
Chen H, Yang B, Shuang X, Zhang T, Meng XY, Ng WK, Yang YL, Wong KS, Chen HN, Yang SH (2017) Tuning the A-site cation composition of FA perovskites for efficient and stable NiO-based p-i-n perovskite solar cells. J Mater Chem A 5:21858–21865
Kim HS, Park NG (2014) Parameters affecting I-V hysteresis of CH3NH3PbI3 perovskite solar cells: effects of perovskite crystal size and mesoporous TiO2 layer. J Phys Chem Lett 5:2927–2934
Li YL, Sun WH, Yan WB, Ye SY, Peng HT, Liu ZW, Bian ZQ, Huang CH (2015) High-performance planar solar cells based on CH3NH3PbI3-xClx perovskites with determined chlorine mole fraction. Adv Funct Mater 25:4867–4873
This work is supported by the NSFC-Henan Province Joint Fund (U1604144), Science Fund of Henan Province (162300410020), Science Project of Education Department of Henan Province (No. 17A140005), Science and Technology Development Project of Henan Province (No. 172102410043), and Program for Science and Technology Innovation Talents in Universities of Henan Province (No. 16HASTIT043).
Availability of Data and Materials
All data are fully available without restriction.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Figure S1. a Survey XPS spectrum of UC-TiO2. b O 1s peak. Figure S2 Scheme of the perovskite solar cells. Figure S3 I-V curves of the devices based on the mesoporous layers without UC-TiO2 and with UC-TiO2 measured under the simulated solar radiation in the wavelength range of λ ≥ 980 nm with a NIR filter. (DOCX 81 kb)
About this article
Cite this article
Zhang, Z., Qin, J., Shi, W. et al. Enhanced Power Conversion Efficiency of Perovskite Solar Cells with an Up-Conversion Material of Er3+-Yb3+-Li+ Tri-doped TiO2. Nanoscale Res Lett 13, 147 (2018). https://doi.org/10.1186/s11671-018-2545-y
- Enhanced power conversion efficiency
- Perovskite solar cells
- Up-conversion material